# Unconventional superconductivity, magnetic and charge order and ...

Unconventional superconductivity, magnetic and charge order and ...

Unconventional superconductivity, magnetic and charge order and ...

### Create successful ePaper yourself

Turn your PDF publications into a flip-book with our unique Google optimized e-Paper software.

ICMR Summer School on Novel Superconductors

M. Brian Maple

Department of Physics

University of California, San Diego

Lecture 1 (Tuesday, 8/11/09):

Interplay between **superconductivity** **and** magnetism in

f-electron systems

(conventional **superconductivity**)

Lecture 2 (Wednesday, 8/12/09):

**Unconventional** **superconductivity**, **magnetic** **and** **charge** **order**,

**and** quantum criticality in heavy fermion f-electron materials

(unconventional **superconductivity**)

• f-electron materials – multinary compounds **and** alloys containing rare earth

(R) **and** actinide (A) ions with partially-filled f-electron shells **and** localized

**magnetic** moments

• Localized **magnetic** moments of R **and** A ions interact with the momenta **and**

spins of the conduction electrons

• Certain R ions (Ce, Pr, Sm, Eu, Tm, Yb) **and** A ions exhibit valence

instabilities; i.e., localized f-states hybridize with conduction electron states

• Competing interactions — readily “tuned” by x, P, H (“knobs”)

• Wide variety of correlated electron phenomena

– Rich **and** complex phase diagrams in the hyperspace of T, x, P, H

• Situations involving competing interactions

– One phenomenon survives at the expense of another

– Interactions conspire to produce a new phenomenon (e.g., sinusoidallymodulated

**magnetic** state that coexists with SC in FM superconductors)

• Brief survey – point of view of experimentalist

• Materials driven physics!

f-electron materials

• Materials – reservoir of new electronic states **and** phenomena

• Opened up new research directions in condensed matter physics

f-electron materials

Lecture 1;Lecture

2

Examples

• Destruction of SC at T c2

< T c1

(reentrant SC) due to Kondo effect

• Kondo effect (impurities **and** lattice)

• Destruction of SC at T c2

< T c1

(reentrant SC) due to FM **order**

• Occurrence of sinusoidally modulated **magnetic** state ( ~ 100 Å) that

coexists with SC in FM superconductors

• Coexistence of SC & AFM **order**

• Coexistence of SC & itinerant FM

• Magnetic field induced SC (MFIS)

• Heavy fermion compounds (m* ~ 10 2 m e

)

• **Unconventional** SC in heavy fermion compounds

– Electron pairing with L > 0, nodes in SCing energy gap, **magnetic**

pairing mechanism

• Occurrence of SC near **magnetic** QCPs accessed by pressure

• NFL behavior associated with QCPs

• Heavy fermion behavior **and** SC in PrOs 4

Sb 12

, possibly due to electric

quadruple, rather than **magnetic** dipole, fluctuations

Lecture 1:

Lecture outlines

Interplay between **superconductivity** **and** magnetism in

f-electron systems

Outline:

(1) f-electron materials

(2) Conventional **superconductivity**

(3) Magnetic interactions in superconductors

(4) Para**magnetic** impurities in superconductors

(5) Magnetic field induced **superconductivity** (MFIS)

(6) Magnetic **order**ing via the RKKY interaction

(7) Magnetically **order**ed superconductors

Lecture outlines

Lecture 2:

**Unconventional** **superconductivity**, **magnetic** **and** **charge** **order**,

**and** quantum criticality in heavy fermion f-electron materials

Outline:

(1) **Unconventional** **superconductivity**

(2) Heavy fermion compounds

(3) Superconductivity in heavy fermion compounds

(4) Competition between Kondo effect **and** RKKY interaction

(5) Non-Fermi liquid (NFL) behavior **and** quantum criticality

(6) SC near antiferro**magnetic** (AFM) quantum critical points (QCPs)

under pressure

(7) Coexistence of SC **and** itinerant ferromagnetism

(8) Heavy fermion behavior **and** unconventional SC in PrOs 4 Sb 12 ;

evidence for electron pairing via electric quadrupole interactions

Some remarks about heavy fermion

f-electron materials

f-electron materials & hybridization

• Hybridization of localized f- & conduction-electron states

interesting correlated electron physics!

• Hybridization strength:

Weak ionic behavior (f occupation number integral)

Moderate Kondo behavior ( ~integral)

Appreciable Valence fluctuations ( nonintegral)

Strong f-b**and**s

• Competing interactions & coupling between

spin, **charge**, lattice degrees of freedom

Novel electronic ground states & phenomena

– Magnetic & quadrupolar **order**

– Valence fluctuations

– Heavy fermion behavior

– Hybridization gap semiconductivity (Kondo insulator behavior)

– Non-Fermi liquid behavior

– **Unconventional** (p- or d-wave) **superconductivity**

f-electron materials & hybridization

• Complex phase diagrams in the hyperspace of

T, P, H, composition

• Systems with quantum critical point (QCP):

– QCP: value of control (tuning) parameter (e.g., composition x,

P, H) where 2 nd **order** phase transition suppressed to 0 K

(quantum phase transition)

– Fluctuations or **order** parameter (**magnetic**, quadrupolar) lead to

breakdown of L**and**au Fermi liquid theory & to formation of other

phases such as glassy types of **magnetic** **order** & unconventional

**superconductivity**

• Materials:

CeIn 3 , Ce(Rh 1-x Co x )In 5 , PrOs 4 Sb 12 ,

UGe 2 , Sc 1-x U x Pd 3 , URu 2-x Re x Si 2

Heavy fermion f-electron materials

Underlying physics — significant hybridization between

localized f- & conduction-electron states

• AFM exchange interaction

H ex = - 2JSs where J ~ -/(E F -F f ) < 0

• Kondo effect (lattice of Ln, U ions)

T K ~ T F exp(-1/N(E F )|J|) ~ T* (effective T F )

• T >> T*: local moment behavior

(T) ~ N eff2 /3k B (T+T*)

(T) ~ - lnT

• T

Kondo effect vs RKKY interaction

Doniach phase diagram

Temperature

T K exp(-1/|J|N(E F ))

T RKKY

J 2 N(E F

)

T N

AFM

NFL

QCP

|J|N(E F )

Heavy fermion f-electron materials

Superconductivity

• Pairing of electrons with L > 0

L=1 (p-wave), S=1 (triplet)

L=2 (d-wave), S=0 (singlet)

• Pairing mechanism — spin fluctuations

• Anisotropic energy gap (k) const.

(k) vanishes at points or lines on Fermi surface

• Superconducting properties ~ T n for T

Non-Fermi liquid behavior

• Materials: U, Ce, Yb intermetallic compounds

– Chemically substituted: Y 1-x U x Pd 3 , UCu 5-x Pd x , CeCu 6-x Au x ,…

– Stoichiometric: (P=0) – UBe 13 , CeCoIn 5 ,YbRh 2 Si 2 ,…;

(P>0) – CeIn 3 , CePd 2 Si 2 ,…

• Physical properties — weak power law, logarithmic divergences in T

at low T

Non-Fermi liquid behavior

Experiments two routes to NFL behavior:

(1) Single ion & (2) inter-ionic interactions

(1) Single ion models

• Multichannel Kondo effect

• Single channel Kondo effect with dis**order** — P(T K )

(2) Interacting ion models

• Fluctuations of **order** parameter

above 2 nd **order** phase transition at 0 K

• Griffiths’ phase — interplay between dis**order** &

competing Kondo **and** RKKY interactions

Superconductivity near **magnetic** QCP apparently

mediated by spin fluctuations

• General overview heavy fermion **and** non-Fermi liquid behavior in f-electron

systems with examples

• Recurring theme: interplay between SC **and** **charge** or spin **order**

o A few examples of SC occurring in the vicinity of phase boundaries for

**charge** or spin **order** that suggests that the **order**ed phase is involved in

the SC

• Several possible scenarios:

– SCing electron pairing mediated by fluctuations of an **order**

parameter near quantum critical point (QCP)

– Liberation of the SCing phase through the suppression of the

**order**ed phase which competes with SC

– Direct participation of the **order**ed phase in the SCing electron

pairing

o Transition metal oxypnictides (SDW)

o Lanthanide tritellurides (CDW)

o URu 2

Si 2

(“hidden **order**” DW phase, various **magnetic** **and** NFL phases)

o SC of the elements

This talk

Heavy fermion superconductors

Electrical resistivity of selected heavy fermion compounds

After Fisk, Ott, Rice & Smith 86

Magnetic susceptibility of selected heavy fermion compounds

After Fisk, Ott, Rice & Smith 86

C/T = vs T 2 for CeCu 2 Si 2 , UBe 13 , **and** UPt 3

C e (T) = (T)T

(0) ≈ 1 J/mol-K 2

Fermi liquid aspects of heavy fermion metals

Wilson-Sommerfeld ratio R:

R = (/)( 2 k B2 / eff2 ); eff2 = g J2 B2 J(J+1)

R ≈ 1 for free electrons

Fermi liquid (L**and**au)

= C/T ~ m* ~ 1/T*

~ m*/(1+F oa )

= AT 2 ~ (T/T*) 2 ~ 2 T 2

Electron-electron scattering

Heavy quasiparticles:

el-el (T) ~ AT 2 ~ (T/T*) 2 ~ 2 T 2

A ~ 2 ,lnA 2ln

Kadowaki-Woods plot

Heavy fermion superconductors

*

*

*

*

*

*

T c (K)

CeCoIn 5

2.3

CeCu 2 Si 2

0.49

CeIrIn 5

0.4

U 6 Fe 3.7

UPd 2 Al 3

2.0

URu 2 Si 2

1.5

UNi 2 Al 3

1.0

UBe 13

0.85

UPt 3

0.55

URhGe 0.4

PuCoGa 5

18

PrOs 4 Sb 12

1.8

Magnetic **order**

Heavy fermion superconductors

*

*

*

*

*

*

T c (K)

CeCoIn 5

2.3

CeCu 2 Si 2

0.49

CeIrIn 5

0.4

U 6 Fe 3.7

UPd 2 Al 3

2.0

URu 2 Si 2

1.5

UNi 2 Al 3

1.0

UBe 13

0.85

UPt 3

0.55

URhGe 0.4

PuCoGa 5

18

PrOs 4 Sb 12

1.8

Superconducting under pressure:

*

*

*

*

*

*

*

T c (K)

CeRhIn 5

2.2 21

Ce 2 RhIn 8

2 23

CeCu 2 Ge 2

~2 165

CePd 2 Si 2

0.43 28

CeRh 2 Si 2

0.26 11

CeNi 2 Ge 2

0.23 23

CeIn 3 0.17 25

UGe 2

0.7 10

Magnetic **order**

P (kbar)

C/T vs T 2 for UBe 13

(0) ≈ 1 J/mol-K 2

m* ~ 10 2 m e

C ≈ T c

Origin: Kondo effect

CeCoIn 5 : heavy fermion superconductor

H = 0:

Superconductivity

H = 50 kOe:

NFL behavior

C Petrovic et al., J. Phys.: Condens. Matter 13 (2001) L337

Upper critical field H c2 (T) of UBe 13

M. B. Maple et al. (85)

H c2 (T) for conventional superconductor

H c2

T

Multiple superconducting phases in U 1-x Th x Be 13

R. H. Heffner et al., PRL 65 (90)

S. E. Lambert et al., PRL 57 (86)

Power law T-dependence of superconducting properties

of heavy fermion superconductors UBe 13 **and** UPt 3

After Fisk, Ott, Rice & Smith 86

Multiple superconducting phases in UPt 3

Two distinct SCing transitions

(sensitive to H & P)

Hasselbach, Taillefer, Flouquet 89

Coupling between multicomponent

SCing OP & AFM OP

AFM: T N ≈ 5 K

≈ 0.02 B /U (basal plane)

Aeppli et al. 88

H – T phase diagram of UPt 3

Ultrasonic velocity measurements

Adenwalla, Ketterson, Yip, Lin, Levy, Sarma 92

B-phase: odd-parity,

spin-triplet SCing state

Sauls ‘94

Multiple superconducting phases in U 1-x Th x Be 13

H. R. Ott et al. PRB 31 ‘85

R. H. Heffner et al. PRL 65 ‘90

Multiple superconducting phases in U 1-x Th x Be 13

R. H. Heffner et al. PRL 65 ‘90

S. E. Lambert et al. PRL 57 ‘86

High temperature **superconductivity** in PuCoGa 5

Sarrao et al. ‘02

Non-Fermi liquid behavior in f-electron systems

Non-Fermi liquid behavior in M 1-x U x Pd 3 (M = Y, Sc) systems

Y 1-x U x Pd 3 : First f-electron system in which NFL behavior observed

C. L. Seaman, M. B. Maple, B. W. Lee, S. Ghamaty, M. S. Torikachvili,

K. N. Yang, L. Z. Liu, J. W. Allen, D. L. Cox, PRL 67, 2882 ’91

(T,H), C(T), M(T,H) for 0 < x ≤ 0.2

Interpreted NFL behavior in terms of quadrupolar Kondo effect

B. Andraka, A. M. Tsvelik, PRL 67, 2886 ‘91

(T,H), C(T,H), M(T,H) for x = 0.2

Interpreted NFL behavior in terms of OP fluctuations

associated with **magnetic** transition suppressed to 0 K

Extensive investigations situation much more complex

INS studies: U 4+ energy level scheme in cubic CEF not yet established

Fluctuations in U concentration x on ~10 m scale (S. Süllow et al. ‘91)

Sc 1-x U x Pd 3 : NFL behavior similar to that observed in Y 1-x U x Pd 3 system

More homogeneous distribution of U

INS studies: /T scaling of ’’(,T)

Interplay between Kondo effect, dis**order**, AFM interactions

T-x phase diagram of Y 1-x U x Pd 3 system

C. L. Seaman et al., PRL 67, 2882 ‘91

D. A. Gajewski, N. R. Dilley, R. Chau, M. B. Maple, J. Phys.: Condens. Matter 8, 9793 ‘96

Electrical resistivity vs T for the Y 1-x U x Pd 3 system (high T)

M. B. Maple, R. P. Dickey, J. Herrmann, M. C. de Andrade, E. J. Freeman,

D. A. Gajewski, R. Chau, J. Phys.: Condens. Matter 8, 9773 ‘96

Low-T NFL behavior in (T), C(T), (T) for Y 1-x U x Pd 3

(T

T-x phase diagrams & low T properties of M 1-x U x Pd 3 (M = Y,Sc)

• Similar T-x phase

diagrams & low T

NFL characteristics

in (T), C(T)/T, (T)

• T K

decreases with x

• AFM & SG phases

• SG QCP

M=Y: x c

≈ 0.2

M=Sc: x c

≈ 0.3

• NFL behavior

associated with

SG QCP

D. A. Gajewski, R. Chau, M. B. Maple, PRB 62, 5496 ‘00

Inelastic neutron scattering on Sc 1.65 U 0.35 Pd 3 : /T scaling

’’(q,,T) = 1/[AT F(/T)]

with = 1/5

No q-dependence no

evidence for U-U correlations

Single impurity critical scaling

associated with spin glass

transition suppressed to 0 K

Solid line: F(/T) = exp[(1/2 – i/2T)]

Proposed for AFM QCP — Q. Si et al., Nature 413, 804 ‘01

S. D. Wilson, P. Dai, D. T. Androja, S.-H. Lee, J.-H. Chung,

J. W. Lynn, N. P. Butch, M. B. Maple, PRL ‘05 (in press)

Inelastic neutron scattering on Sc 1.65 U 0.35 Pd 3 : /T scaling

Similar behavior: ’’(q,,T) 1/AT F(/T)

UCu 5-x Pd x (x = 1, 1.5); = 1/3

Near AFM QCP

M. Aronson et al., PRL 75, 725 ‘95; PRL 87,197205 ‘01

CeCu 5.9 Au 0.1 ; = 0.75

A. Schröder et al., PRL 80, 5623 ‘98

Near AFM QCP

Absence of energy scale, other than T itself

Microscopic origin of the NFL behavior involves

individual ions near 0 K spin glass phase transition

Although impurities may play role, they do not

appear to be primary cause

T-x phase diagrams for U 1-x M x Pd 2 Al 3 (M = Th, Y, La)

NFL behavior in U 1-x Y x Pd 2 Al 3

near QCP at x c ≈ 0.65

UCSD ‘01

Superconductivity near quantum critical points

Superconductivity near pressure-induced AFM QCP

AFM QCP:

P c ≈ 28 kbar

(T) ≈ o + AT 1.2

T c ≤ T ≤ 40 K

T c (max) ≈ 0.4 K

Similar behavior

for CeIn 3 under P

Julian, Lonzarich et al. (98)

Suggests AFM spin fluctuations responsible for

NFL behavior in (T) **and** SCing electron pairing

Superconductivity within the ferro**magnetic** state in UGe 2

• First P-induced FM-SC

Saxena et al. (00)

High purity crystal (l >>

microscopic coexistence

of triplet-spin SC & FM?

• Itinerant electron FM

C

= 53 K (P = 0)

• ≈ 35 mJ/mol K 2

m* ≈ 20 m e

Onuki et al. (93)

• C

0 K at P c

≈ 16 kbar

Oomi et al. (98)

• Experiments on polycrystalline UGe 2

(l ≈ )

Inhomogeneous state: coexistence of

singlet-spin SC regions & FM regions?

Bauer, Zapf, Ho, Maple (01)

Crystal structure of filled skutterudites

Filled skutterudites: MT 4 X 12 (M = alkali metal, alkaline earth, rare earth,

actinide; T = Fe, Ru, Os; X = P, As, Sb)

Binary skutterudites: TX 3 (T = Co, Rh, Ir; X = P, As, Sb)

Prototype CoAs 3 : Discovered in Skutterud, Norway

M cations — bcc sublattice

(atomic cages — undergo large

amplitude vibrations)

T cations — sc sublattice

X anions — distorted corner

sharing octahedra centered

by T cation

bcc structure (Im-3)

a = 9.3068 Å

W. Jeitschko & D. J. Braun 77

PrOs 4

Sb 12

Heavy fermion superconductor PrOs 4 Sb 12

AFQO

Pr 3+ energy levels in CEF

INS measurements

Goremychkin et al., 04

Ho et al., 03

3

doublet (~200 K)

4

triplet (~130 K)

5

triplet (~7 K)

1

singlet (0 K)

• First Pr-based heavy fermion (HF)

superconductor (SC)

(m* ~ 50 m e ; T c = 1.85 K)

Bauer et al., 01; Maple et al., 02

• **Unconventional** type of strongcoupling

SC

• Evidence for several distinct

SCing phases, point nodes in (k),

time reversal symmetry breaking

• Possible c**and**idate for triplet SC

• Evidence for multib**and** SC

Sayfarth et al., 06

• HFOP identified with antiferroquadrupolar

**order** (AFQO):

neutron diffraction Kohgi et al., 03

• SC in vicinity of AFQ QCP!

• HF behavior **and** unconventional

SC may be mediated by electric

quadrupole fluctuations

• Off-center rattling **and** tunneling of

Pr filler ion may play role in HF

behavior **and** SC

Goto et al., 04

High temperature **superconductivity** **and** spin density

waves in transition metal pnictides

High temperature **superconductivity** **and** spin density waves in

transition metal pnictides

Coworkers

University of California, San Diego

R. E. Baumbach, N. M. Crisosto, J. J. Hamlin, T. A. Sayles, L. Shu, D. A. Zocco

D. N. Basov, M. M. Qazilbash

Oak Ridge National Laboratory

R. Jin, D. M**and**rus, M. A. McGuire, B. C. Sales, A. S. Sefat

D. J. Singh, Lijun Zhang

Lawrence Livermore National Laboratory

J. R. Jeffries, S. T. Weir

University of Alabama, Birmingham

Y. K. Vohra

Superconductivity in transition metal pnictides

• Recent developments in high T c **superconductivity**

– LnFeAsO 1-x F x

• Maximum T c ≈ 55 K (Ln = Sm)

• Structure type: ZrCuSiAs (1:1:1:1)

– A 1-x M x Fe 2 As 2

• Maximum T c ≈ 38 K (A = Sr, M = K, Cs; A = Ba, M = K)

• Structure type: ThCr 2

Si 2

(1:1:2) (structure of many HF SCs)

• Superconductivity

– Periodically declared to be “all over”

– Resuscitated by developments in materials; e.g.,

• Magnetic superconductors (~75)

• Organic superconductors (~75)

• Heavy fermion superconductors (~80)

• High T c cuprate superconductors (~86)

• High T c transition metal pnictide superconductors (~08)

Highest T c achieved vs year

Iron-pnictide high-temperature superconductors

Journal of Alloys **and** Compounds 302 (2000) 70–74

Wolfgang

Jeitschko

LaFePO

LaFePO 1-x

F x

T c

~3 K

T c

~ 5 K

LaFePO

LaFePO 1-x

F x

T c

~ 3 K

T c

~ 5 K

Structure of LaFeAsO

La

Fe

As

O

• Tetragonal ZrCuSiAs prototype

• Edge sharing FeAs 4

tetrahedra

• Fe atoms form square nets

• Fe-Fe bonding likely to be important

• a = 4.034 Å, c = 8.745 Å

Structure of TM pnictide 1:1:1:1 **and** 1:2:2 superconductors

Structure type: ZrCuSiAs

Structure type: ThCr 2

Si 2

K. Sasmal, B. Lv, B. Lorenz, A. Guloy, F. Chen,

Y. Xue, C. W. Chu, arXiv:0806.1301 (2008)

LaFeAsO 1-x F x

CeFeAsO 1-x F x

NdFeAsO 1-x F x

SmFeAsO 1-x F x

26 K

40 K

50 K

55 K

Ba 1-x K x Fe 2 As 2

Ca 1-x Na x Fe 2 As 2

38 K

40 K

Transition metal-pnictogen structures

FeTe “11”

SrFe 2

As 2

“122”

PrFeAsO

“1111”

LiFeAs “111”

LnFeAsO 1-x F x high T c superconductors

SmFeAsO 1-x

F x

LaFeAsO 1-x

F x

Nomura et al. arxiv:0804.3569

Liu et al. arxiv:0804.2105

SDW **and** SC under pressure SrFe 2 As 2

Tou et al., arXiv: 0810.4856v1 (08)

Superconductivity in LaFePO

J. J. Hamlin, R. E. Baumbach, D. A. Zocco,

T. A. Sayles, M. B. Maple, JPCM 20, 365220 (08)

• LaFePO single crystals grown

in Sn flux

• Superconductivity: T c

= 6.7 K

• Significant anisotropy of

resistively determined H c2

(T)

curves

Superconductivity in LaFePO

T c

• No measurable jump in C(T) at T c

= 6.7 K

• Very small superconducting fraction?

• Superconductivity due to oxygen defects?

J. J. Hamlin, R. E. Baumbach,

D. A. Zocco, T. A. Sayles,

M. B. Maple, JPCM 20, 365220 (08)

Superconductivity in LnFePO (Ln = La, Pr, Nd)

LnFePO (Ln = La, Pr, Nd)

• T c

lower for Ln = Pr, Nd

• Metallic behavior

• No evidence for SDW

• ≈ T 2 for 10 K < T < 100 K

• Large RRR values

Ln

T c

(K) RRR

La 6.6 32

Pr 3.2 14

Nd 3.1 28

R. E. Baumbach, J. J. Hamlin, L. Shu, D. A. Zocco,

N. M. Crisosto, **and** M. B. Maple, NJP 11, 025018 (09)

O 2

annealing for LnFePO (Ln = La, Pr, Nd)

• Unannealed PrFePO **and**

NdFePO show nearly zero

shielding

• O 2

annealing improves

shielding for PrFePO **and**

NdFePO

• O 2

annealing slightly

increases T c

for LaFePO

R. E. Baumbach, J. J. Hamlin, L. Shu, D. A. Zocco,

N. M. Crisosto, **and** M. B. Maple, NJP 11, 025018 (09)

C(T) for LnFePO (Ln = La, Pr) single crystals

• No specific heat jump for as-grown

LaFePO **and** PrFePO

• Specific heat jump observed for O 2

annealed PrFePO

• Jump is nearly 100 % of value

expected from BCS for O 2

annealed PrFePO

• Schottky anomaly for PrFePO

• CEF fits suggest non**magnetic**

ground state **and** first excited

state: ~ 41 K

R. E. Baumbach, J. J. Hamlin, L. Shu, D. A. Zocco,

N. M. Crisosto, **and** M. B. Maple, NJP 11, 025018 (09)

• Annealing sharpens CEF peak –

may indicate reduced spread

of CEF splittings

• Small for LaFePO **and** PrFePO

Comparison of T c

vs Ln for Pn = P, As

• Solid circles: LnFeAsO 1-x

F x

• Open circles: LnFeAsO 1-x

• Solid squares: LnFePO

• Much lower T c

for Pn = P

• For Pn = As: T c

enhanced

with **magnetic** Ln

• For Pn = P: T c

depressed

with **magnetic** Ln

• Possible **magnetic** pairbreaking

for LnFePO

R. E. Baumbach, J. J. Hamlin, L. Shu, D. A. Zocco,

N. M. Crisosto, **and** M. B. Maple, NJP 11, 025018 (09)

• Suggests that arsenides may

be unconventional SCs, while

phosphides are conventional

(BCS) superconductors!

Ratio of kinetic energy from experiment **and** b**and** theory K exp /K b**and**

for iron pnictides **and** various other materials

Infrared **and** optical study of

electronic correlations in LaFePO

M. M. Qazilbash, J. J. Hamlin, R. E. Baumbach, Lijun Zhang,

D. T. Singh, M.B. Maple amd D. N. Basov, Nature Physics (09)

Designer Diamond Anvils

blank diamond deposit circuit CVD diamond re-grind diamond

(T, P) for LaFePO

• Dome-shaped T c

(P) curve

• T c, max ~ 14 K

• Similar behavior of T c (P) for

optimally doped LaFeAsO 1-x

F x

**and** CeFeAsO 1-x

F x

• Reminiscent of T c (x) in cuprates

**and** T c

(P) in heavy fermion

f-electron compounds

J. J. Hamlin, R. E. Baumbach, D. A. Zocco,

T. A. Sayles, M. B. Maple, JPCM 20, 365220 (08)

J. J. Hamlin et al. JPCM (08)

APS March Meeting 2009, Ryan E. Baumbach

Oxypnictide superconductors: pressure dependence of T c

D. A. Zocco, J. J. Hamlin, R. E. Baumbach, M. B. Maple,

M. A. Maguire, B. C. Sales, A. S. Sefat, R. Jin, D. M**and**rus,

J. R. Jeffries, S. T. Weir, Y. K. Vohra, J. Superconductivity 08

J. J. Hamlin, R. E. Baumbach, D. A. Zocco,

T. A. Sayles, M. B. Maple, J. Phys.: Cond. Matt. 08

• Dome-shaped dependence of T c

on P

• Reminiscent of T c

vs x in cuprates **and**

T c

vs P in heavy fermion compounds

Electrical resistivity of CeFeAsO under pressure

D. A. Zocco, J. J. Hamlin, M. B. Maple, unpublished (09)

Okada et al., JPSJ 77, 113712 (2008)

arXiv:0903.2143 (2009)

Superconductivity at 17K in Sr 4

Sc 2

Fe 2

P 2

O 6

: new superconducting

layered oxypnictides with thick perovskite oxide layer

Ogino et al., arXiv:0903.3314

Interplay of superconducting, **charge** density wave, **and**

**magnetic** **order** in rare earth tritelluride RTe 3 compounds

Interplay of superconducting, **charge** density wave, **and** **magnetic** **order**

in rare earth tritelluride RTe 3 compounds

Coworkers

University of California, San Diego

J. J. Hamlin, T. A. Sayles, D. A. Zocco

Stanford University

J.-H. Chu, I. R. Fischer

“2D” **charge** density waves

RTe 3

• Kim et al., PRL 96, 226401 (2006)

• Ru et al., PRB 77, 035114 (2008)

Rare earth tritellurides: RTe 3

• T CDW1 decreases **and** T CDW2

increases with decreasing a

• Suggests similar dependence

of T CDW1 **and** T CDW2 on P

(T) measurements under P

E. DiMasi, M. C. Aronson, J. F. Mansfield, B. Foran, S. Lee, PRB 52,14516 (1995)

N. Ru, I. R. Fisher, PRB 73, 033101 (2006)

J. Lavarock, S. B. Dugdale, Zs. Major, M. A. Alam, N. Ru, I. R. Fisher, G. Santi, E. Bruno, PRB 71, 0851144 (2005)

N. Ru, J. -H. Chu, I. R. Fisher, PRB 78, 012410 (2008)

SCing, CDW, **and** AFM **order** under pressure in TbTe 3

J. J. Hamlin, D. A. Zocco,

T. A. Sayles, M. B. Maple,

J.-H. Chu, I. R. Fischer, 08

• Interplay of CDW, AFM & SC

• P-induced SC

• CDW, AFM, SC coexist (~23 kbar)

• Opportunity to study **magnetic**ally

**order**ed SCs under P

Evidence for antiferro**magnetic** **order**ing of Tb 3+ ions in TbTe 3

J. J. Hamlin, D. A. Zocco, T. A. Sayles,

M. B. Maple, J.-H. Chu, I. R. Fischer, 08

Interplay of hidden, **magnetic**, **and** superconducting

**order** in URu 2 Si 2

Coworkers

University of California,

San Diego

N. P. Butch U. Maryl**and**

J. R. Jeffries Lawrence Livermore National Laboratory

T. A. Sayles Quantum Design, San Diego

B. T. Yukich UCSD, SOM

D. A. Zocco

• Delicate interplay between competing interactions in URu 2

Si 2

produces a wide

variety of correlated electron phenomena

• Phenomena include

– Superconductivity (SC)

– A “hidden **order**” (HO) phase that apparently forms a gap over portion of

Fermi surface (like SDW or CDW)

– Antiferromagnetism (AFM)

– Ferromagnetism (FM)

– Heavy fermion (HF) behavior

– Non-Fermi liquid (NFL) behavior

URu 2-x Re x Si 2 : Introduction

• Interactions “tuned” via P, H, chemical substitution

• Experiments on suppression of HO phase **and** onset of FM in URu 2

Si 2

via Re

substitution — objectives:

– Investigate physical properties of single crystals of URu 2-x

Re x

Si 2

(0 ≤ x ≤ 1)

– Allows the anisotropy of physical properties to be determined — advantage

over previous studies on polycrystalline specimens of URu 2-x

Re x

Si 2

– Establish T-x phase boundaries **and** locations of quantum phase transitions

(QPTs) for HO **and** FM phases

– Characterize NFL behavior associated with quantum critical points (QCPs)

URu 2 Si 2 : Initial experiments

• Heavy fermion **superconductivity** (polycrystalline specimens)

Schlabitz, Baumann, Pollit, Rauchschwalbe, Mayer, Alheim, Bredl, ZP (86)

• Anisotropy of physical properties (single crystal specimens)

Palstra, Menovsky, van den Berg, Dirkmaat, Kes, Nieuwenhuys, Mydosh, PRL (85)

• Partial gapping of the FS by CDW or SDW (polycrystalline specimens)

Maple, Dalichaouch, Kohara, Rossel, Torikachvili, McElfresh, Thompson, PRL (86)

• SM-AFM – neutron scattering experiments (single crystal specimens)

Broholm, Kjems, Buyers, Matthews, Palstra, Menovsky, Mydosh, PRL (86)

• Followed by an enormous amount of experimental **and** theoretical work,

especially devoted to establishing the identity of the so-called “hidden

**order**” phase

• Review some of history that led us to the Re substitution experiments in URu 2

Si 2

Why URu 2 Si 2 is interesting

ThCr 2

Si 2

structure

a = 4.13 Å, c = 9.58 Å

• Moderately heavy Fermi liquid (m* ~ 25 m e

)

• “Hidden **order** (HO)” phase (T 0

≈ 17.5 K)

• BCS-like feature in C(T) at 17.5 K suggests partial

gapping of Fermi surface by CDW or SDW

• Small moment antiferromagnetism (SM-AFM):

≈ 0.03 B

/U, ||c-axis, (100) modulation

• S ≈ 0.2ln(2) too large “HO” phase

• Large moment antiferromagnetism (LM-AFM)

observed at P c

~ 5 - 15 kbar: ~ 0.4 B

/U

• SM-AFM phase – small volume fraction of LM-AFM

phase that coexists with HO phase av

≈ 0.03 B

• Is HO/LM-AFM phase separation due to strain?

• Superconductivity (SC) (T c

≈ 1.5 K)

• Coexists with HO **and** SM-AFM phases

• Ordered phases can be “tuned” with P, H, x:

• Produces LM-AFM (Rh) **and** LM-FM (Re) phases

• Non-Fermi liquid (NFL) behavior

Low temperature specific heat of URu 2 Si 2

SCing transition

C’(T)/T=’+T 2

’

(0)

C(T)/T=+T 2

Maple, Dalichaouch, Kohara, Rossel, Torikachvili,

McElfresh, Thompson, PRL (86)

• BCS-type mean field transition at T o

= 17.5 K

– C ≈ Aexp(-/T); ~ 10 2 K SDW or CDW

– (0)/’ ≈ 0.6 ~ 40 % Fermi surface removed by SDW or CDW

– SC & SDW or CDW compete for Fermi surface!

• S ≈ 0.2ln(2) too large for AFM with small ≈ 0.03 B

Hidden **order** (HO)?

• Superconductivity below T c

≈ 1.5 K (onset)

Effect of pressure on competing electronic states in URu 2 Si 2

McElfresh, Thompson, Willis, Maple,

Kohara, Torikachvili, PRB (87)

Superconductivity under pressure – T c (P) & H c2 (T,P)

URu 2

Si 2

single crystal

Phenomenological fits to H c2 (T) data:

H c2 (T) = H c2 (0)[1 - A(T/T c ) 2 ]

No features in T c

(P) **and** H c2

(T,P) curves to ~15 kbar

no qualitative change in SC due to onset of LM-AFM phase near 5 kbar!

J. R. Jeffries, N. P. Butch, B. T. Yukich, M. B. Maple, PRL (07)

Low temperature specific heat of URu 2 Si 2 under pressure

R. A. Fisher, S. Kim. Y. Wu,

N. E. Phillips, M. W. McElfresh,

M. S. Torikachvili, M. B. Maple (90)

NOTE: Rapid reduction of specific

heat jump C at T c with P

Two possible interpretations:

(1) Suppression of SCing volume

fraction to immeasurably small

value by ~ 5 kbar;

(2) Manifestation of unconventional

nature of SC

URu 2 Si 2 : HO – LM-AFM phase transition under P

Neutron diffraction: AFM

increases with P

29

Si NMR: phase separation –

AFM volume increases with P

(HO volume decreases with P)

~0.4 B

P c ≈ 15 kbar

AFM

~0.03 B

PM

H. Amitsuka et al., PRL (99) K. Matsuda et al., JP:CM (03)

URu 2 Si 2 : Possible T-P phase diagrams

Knebel et al., JMMM (07)

Amitsuka et al., JMMM (07)

• Left h**and** T – P phase diagram favored by continuous behavior of T c

(P)

**and** H c2

(T,P)

• Right h**and** T – P phase diagram could be favored if rapid diminution of

C at T c

near 6 kbar signals loss of bulk SC

• There appears to be a steep (vertical?) phase boundary at P c

≈ 15 kbar

(nearly independent of T - red line in figures)

• HO – LM-AFM phase boundary or another phase boundary?

Field-induced phases in URu 2 Si 2

Electrical resistivity

= o

+ AT n

n = 2: FL

n ≈ 1 - 1.5: NFL

K. H. Kim et al., PRL 91 ‘03

URu 2-x Re x Si 2 : FM **and** NFL behavior

Relation

to NFL?

• NFL features in (T), C(T) not clearly peaked at x = 0.15

• Extend deep into FM state

• 3D itinerant FM QCP:

• (T) ~ T 5/3

• C(T)/T ~ -lnT

• (T) ~ T 3/4

• T C

~ (x - x c

) 3/4

• Quantum Griffith’s phase scenario:

• (T) ~ C(T)/T ~ T -1

Comparison of URu 2-x M x Si 2 (M = Rh, Re) phase diagrams

Kawarazaki et al., JPSJ (94)

Yokoyama et al., JPSJ (04)

This work

Superconductivity in pure elemental solids

Field-induced phases in pure **and** Rh substituted URu 2 Si 2

URu 2 Si 2 URu 2-x Rh x Si 2

URu 2-x Re x Si 2

S. Francoul et al.,

(09); this conference

K. H. Kim et al., PRL (03)

K. H. Kim et al., PRL (04)

Electrical resistivity

= o

+ AT n

n = 2: FL

n ≈ 1 - 1.5: NFL

Superconductivity in pure elemental solids

T. Yabuuchi, T. Matsuoka, Y. Nakamoto, K. Shimizu

J. Phys. Soc. Japan, 75, 083703 (2006)

M. Debessai, J. J. Hamlin, J. S. Schilling

arXiv:0806.3407 (submitted to PRB)

END

• Metallic compounds containing Ln & A ions with partially-filled

f-electron shells & unstable valence (no. of f-electrons)

• Lanthanides – Ce, Pr, Yb; actinides – U, Pu

• Hybridization between localized f- & conduction-electron states

• Narrow resonance near the E F

Heavy fermion f-electron materials

• Effective Fermi temperature – T*

• T >> T*: local moment behavior

N(E)

(T) ~ N eff2 /3k B (T+T*)

(T) ~ - lnT

k B T*

• T

H–T phase diagram of PrOs 4 Sb 12

QCP

T. Yanagasawa (06)

QCP

Ho et al., PRB (03)

HFOP

• Related to crossover of

CEF energy levels

• Identified with antiferroquadrupolar

**order**:

neutron diffraction

Kohgi et al., JPSJ (03)

• Anisotropic phase

boundary: M(H,T)

Tayama et al., JPSJ (03)

• SC in vicinity of antiferroquadrupolar

QCP!

Why PrOs 4 Sb 12 is interesting

• 1 st Pr-based heavy fermion superconductor (T c

= 1.85 K)

Bauer, Frederick, Ho, Zapf, Maple, PRB (02)

(All others based on Ce, U, & Pu)

• Non**magnetic** heavy Fermi liquid (m* ≈ 50 m e

)

• **Unconventional** strong coupling **superconductivity**:

– May consist of several distinct SCing phases

– Evidence for nodes in energy gap – Chia et al., PRB (03)

– Breaks time reversal symmetry – Aoki et al., PRL (03)

– Triplet spin **superconductivity**?

• High field **order**ed phase (HFOP): (H,T) – Maple et al., JPSJ (02);

Ho et al., PRB (03); C(H,T) – Aoki et al., JPSJ (02); Vollmer et al., PRL (03);…

• HFOP identified with antiferroquadrupolar **order**, based on

neutron diffraction at high H: Kohgi et al., JPSJ (03)

• SC appears to be near quadrupolar quantum critical point (QCP)

• Formation of heavy Fermi liquid &/or unconventional SCing state may involve

electric quadrupole, rather than **magnetic** dipole, fluctuations

• Off-center rattling & tunneling – Goto et al., PRB (04)

• Multib**and** **superconductivity** – Seyfarth et al., PRL (05)

Heavy fermion **superconductivity** in PrOs 4 Sb 12

Normal state:

C(T) = T +T 3 + C Sch

(T)

≈ 500 mJ/mol K 2 , D

≈ 200 K

1

singlet g.s., 5

triplet 1 st e.s., ≈ 7 K

C Sch

(T) scaled by 0.56

~50% entropy conduction electrons

Superconducting state:

• Analyses of C &

slope of H c2

(T) at T c

confirm large value of

derived from C(T) in

normal state

• Structure in C(T) near T c

:

Two SCing phases?

T c1

≈ 1.85 K, T c2

≈ 1.70 K

Intrinsic effect?

Measson et al., PRB (05)

Bauer, Frederick, Ho,

Zapf, Maple, PRB (02);

Maple et al., JPSJ (02)

PrOs 4 Sb 12 : Possible superconducting phase diagram

T*(H)

T c3

T c2 T c1

PrOs 4 As 12 : H-T phase diagram

• Single crystals: Z.Henkie

• Kondo lattice:

T K

~ 1 K

• Heavy fermion behavior:

~ 1 J/mol-K 2

• Two **order**ed phases:

AFM: Low H

Unknown: High H

AFM structure: Alternating

(100) planes of FMically

**order**ed Pr ’s, oppositely

oriented with one another

Yuhasz et al., PRB (06);

Maple et al., PNAS (06)

PrOs 4 As 12 :C e /T vs T in **magnetic** fields

• C e

(T) data:

UCSD (0 ≤ H ≤ 5 T)

LLNL (6 T ≤ H ≤ 16 T)

• C e

(T) fits:

Resonance level model

K. D. Schotte, U. Schotte,

Phys. Lett. (75)

• Spin: S = 1 (triplet CEF g.s.)

• Level width: =k B

T K

≈ 3.5 K

• Zeeman splitting of

resonances: g B

H

• Similar to behavior of PrFe 4

P 12

Aoki et al., PRB ‘02

PrOs 4 As 12 : (0) vs H

AFM

Unknown **order**

Interplay of hidden, **magnetic**, **and** superconducting **order** in URu 2 Si 2

C’(T)/T=’+T 2

C(T)/T=+T 2

Maple, Dalichaouch, Kohara, Rossel, Torikachvili,

McElfresh, Thompson, PRL (86)

• BCS-type mean field transition at T o = 17.5 K SDW or CDW

– ~ 10 2 K C ≈ Aexp(-/T)

– ~ 40 % of FS removed by SDW or CDW ((0)/’ ≈ 0.6)

– Small AFM ( ≈ 0.03 B /U, ||c-axis, (100) modulation)

– Hidden **order** (HO) phase (S ≈ 0.2ln(2) too large for AFM with small

– SC below T c ≈ 1.5 K coexists with HO **and** AFM

• Inhomogeneous mixture of HO **and** large AFM phases; AFM fraction increases with P

• Identity of HO phase? Inhomogeneous HO/AFM mixture intrinsic? T vs P phase diagram?

Effect of pressure on competing electronic states in URu 2 Si 2

McElfresh, Thompson, Willis,

Maple, Kohara, Torikachvili ‘87

Low temperature specific heat of URu 2 Si 2 under pressure

R. A. Fisher, S. Kim. Y. Wu,

N. E. Phillips, M. W. McElfresh,

M. S. Torikachvili, M. B. Maple, 90

NOTE: Rapid suppression of

specific heat jump C at T c

with P

URu 2 Si 2 : Fermi surface competition

• Bilbro & McMillan PRB (76)

– Theory – CDW/SDW competes with

SCing **order** to gap a simple FS

– HO/SMAFM **and** SCing phases

compete for electrons

• n = 0 / norm

– Amount of FS not gapped by

CDW/SDW

– C(T): n(0) = 0.58, T c0 = 3.9 K

T c0 = T c (P) n(P) T 0 (P) 1-n(P)

M. B. Maple et al., PRL (86); J. R. Jeffries,

N. P. Butch, B. T. Yukich, M. B. Maple, PRL (07)

n(P) calculated from T c & T 0 **and** (P=0)

C(T) measured under P

R. A. Fisher et al., Physica B (90)

URu 2 Si 2 under pressure

Amitsuka et al., JMMM (07)

• T 0 increases

• T c decreases

• μ AFM increases

– 0.03μ B 0.4μ B

– Neutron scattering,

NMR, μSR

– (In)homogeneous

HO/AFM distribution?

– HO AFM 1 st **order**?

– HO/AFM coupled?

Knebel et al., JMMM (07)